Chapter 11

1 / 32

# Chapter 11 - PowerPoint PPT Presentation

Chapter 11. Applications and Processing of Metal Alloys. This is just an extension of the previous chapter…. Hardenability of Steels: The Jominy Test. As usual, everything is standardized!.

I am the owner, or an agent authorized to act on behalf of the owner, of the copyrighted work described.

## Chapter 11

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -
Presentation Transcript
1. Chapter 11 Applications and Processing of Metal Alloys This is just an extension of the previous chapter…

2. Hardenability of Steels: The Jominy Test As usual, everything is standardized! After the Jominy specimen cools to RT, hardness is measured along the main axis of the sample at 1/16” intervals. The resulting H vs. distance is called the “Jominy curve”.

3. Hardenability of Steels Notice the variation of hardness and the cooling rates with the distance from the quenched end. Would the cooling curves vary from steel to steel? What would they depend on? For the exam, you need to know this correlation between cooling rate and resulting microstructures.

4. Hardenability of Steels (cont.) How do you predict the hardenability of a steel by “reading” the Jominy curves? Examples In this graph, we have the opportunity of assessing the effect of certain alloying elements on hardenability while the level of carbon is kept constant (0.40 wt.%)

5. Specialized Heat Treatments Austempering: Used in order to produce a 100% bainitic structure that has a high yield strength. Note that the isothermal treatment is conducted a few degrees above MS. Why? Martempering: Used in order to avoid residual stresses caused by differential cooling (surface, core) in large parts. It forms 100% martensitic structure. Note that the isothermal treatment is conducted a few degrees above MS for short time.

6. Specialized Surface Heat Treatments (Hardening) • Required for: • Wear resistance • When the most severe stresses act only on the surface • To increase the the lifetime of the part subject to cyclic stress • Can be done: • By localized heating and quenching • By modifying the chemical composition on and near the surface: • Carburizing • Nitriding • Carbonitriding • Chromizing, etc. Please, give examples of possible applications

7. Notice how the indentations vary in size Surface Hardening: Carburizing Surface diffusion of carbon in a gas furnace at austenization temperature. Starting material: low or medium carbon steels.

8. Classification of Ferrous Alloys

9. Designation of Steels (AISI / SAE)

10. ASTM Designation of Construction Steels

11. Stainless Steels Corrosion resistant steels Their corrosion resistance is due to the large amount of Chrome present: -more than 12 wt.% Cr The effect of Cr is to form a passive layer or protecting oxide layer of Cr2O3. In first contact with the environment the material oxidizes but the oxide does not progress inside

12. Stainless Steels: Fe-Cr alloys Remember where Fe and Cr are in the periodic table. What do you suspect of both metals?

13. Stainless Steels: The Fe-Cr Phase Diagram

14. Stainless Steels Classification It depends on the microstructural conformation of the steels: • Ferritic Stainless Steels • Martensitic Stainless Steels • Austenitic Stainless Steels

15. Ferritic Stainless Steels From 12 to 30% Cr with small amounts of carbon (0.012-0.20%) Matrix: ferritic (-Fe solution) with fine carbide precipitates. No FCCBCC transformation Most inexpensive stainless steel due to no need for Ni. General application when corrosion resistance is needed. Most common: 430 (17 Cr-0.012 C; UTS: 517 MPa, YS: 345 MPa; : 25% 446 (25 Cr-0.20 C; UTS: 552 MPa, YS: 345 MPa; : 20%

16. Martensitic Stainless Steels From 12 to 17% Cr with amounts of carbon (up to 1.1%) necessary to produce martensite Matrix: martensitic (after quenching and tempering) with carbides. FCCBCT transformation (the -loop in the phase diagram is increased) More expensive due to heat treatment. General application when corrosion resistance needs to be accompanied with very high strength and hardness. Most common: 440 (17 Cr-0.7+ C); UTS: 1828 MPa, YS: 1690 MPa; : 5%

17. Austenitic Stainless Steels From 16 to 25% Cr with Ni (7 to 20%) and very little or no carbon Matrix: austenitic, which allows high formability. The FCC structure is stabilized at room temperature by Ni. See Fe-Ni diagram. Most expensive due to Ni content. Very low carbon is needed to avoid intergranular corrosion. Used when maximum corrosion resistance is needed. Most common: 304 (19 Cr – 10 Ni; UTS: 580MPa; YS: 290MPa; : 55% 316 (18 Cr – 12 Ni; UTS: 500 MPa; YS: 225MPa; : 40%

18. Stainless Steel: The Fe-Ni Phase Diagram

19. Intergranular Corrosion in Austenitic Stainless Steel Even small amounts of carbon favor the formation of M23C6 Chromium depletion in the vicinity of a grain boundary in the austenitic steel:

20. This is an example of tensile test curves obtained for different stainless steels Extract all the information you need to compare differences in mechanical properties among different types of stainless steels.

21. Aluminum Alloys • Main advantage: light weight materials • Other advantages: high electrical and thermal conductivities, good ductility (with some exceptions), easy to melt and cast, versatile mechanical properties. • Main disadvantage (for specific potential applications): low melting points.

22. Classification of Aluminum Alloys Aluminum Association designation: • Wrought Alloys • 1XXX, 2XXX, 3XXX, 4XXX, 5XXX, 6XXX, 7XXX • Cast Alloys • 1XX, 2XX, 3XX, 4XX

23. Most Common Aluminum Cast Alloys • The most common ones contain silicon (series 3XX and 4XX) • This is the reason for their good castability

24. Most Common Aluminum Cast Alloys (cont.) • Used to make parts with complicated forms, some abrasion resistance requirements, low thermal expansion • In a car engine they are everywhere: block, pistons, cilinder heads Recently developed functionally-graded aluminum casting: A390→A356

25. Common Wrought Alloys • Most of them can be hardened by precipitation hardening (series 20XX and 70XX) • This requires solubility of the main alloying elements in Al. They are used in numerous products: 3XXX (Al-Mn based) in beverage can bodies 5XXX (Al-Mg based) in beverage can taps 6XXX (Al with small Mg and Si) in many extruded products (frames, etc.) 7075 (Al-Zn-Mg based) in main structural components in aircrafts 2014, 2024 (Al-Cu based) in fuselages and wings

26. Precipitation Hardening in Al Alloys • Solution and precipitation hardening: • Two subsequent treatments at two different temperatures. • Use the solvus line in the Al-rich side of the phase diagrams to select the solution (solubilizing) temperature. • Appearance of new non-equilibrium intermetallic phases. We can adjust final hardness or mechanical strength by artificially generating obstacles to dislocation movement.

27. Tsol. < Teut Solution treatment in Al alloys Liq. T (Al) L + (Al) L + Θ Θ (Al) + Θ We need to have the alloy constituted by just one phase: the solid solution (Al) SOLVUS Al % X

28. Quenching & Aging (Precipitation Hardening) T Liq. T Quenching Tsol L + (Al) L + Θ (Al) Artificial Aging Θ SOLVUS (Al) + Θ time Al % X Natural Aging Main quenching goal: retain the (Al) solution at room temperature, but supersaturated with atoms of X!

29. Aging or Precipitation Hardening At low aging temp. no stable phase (the one in the phase diagram) appears. Instead, new non-equilibrium phases develop sequentially during the aging process. Tsol Artificial Aging time They show up in a sequence: GP zonesPhase1…  where  is the stable phase. It appears at longer times: overaged structure

30. Tsol Artificial Aging time Precipitation Hardening Structures (cont.) In the Al-Cu system the non-equilibrium phases are called: GP zone ’’’ Heat treatable Al alloys: Al-Cu, Al-Zn, Al-Mg, Al-Ag, ternary Al-Zn-Mg, etc.

31. Precipitation Hardening in Al-Cu Alloys These new phases, GP zones, ’’ and ’ act as obstacles to dislocation motion. Some are more effective than others. Dislocation line t t More energy needed to bow around the obstacles!

32. Precipitation Hardening in Al-Cu Alloys and Their Mechanical Properties This is the effect of precipitation hardening and the precipitation sequence (GP zones ’’  ’  ) on the yield strength and ductility of a AA2014 Al alloy